TABLE 1 Chemical Requirements NOTE—Values are maximum unless otherwise indicated. Grade CZ100 M35-1A M35-2 M30H M25S M30CA N12MV N7M CY40 CW12MW CW6M CW2M CW6MC CY5SnBiM CX2MW CU5MCuC CX2M UNS Num- J02100 J24135 J04020 J24030 J24025 J24130 J30012 J30007 J06040 J30002 J30107 J26455 J26625 J26055 N26022 N08826 N26059 bers Composition, % C, max 1.00 0.35 0.35 0.30 0.25 0.30 0.12 0.07 0.40 0.12 0.07 0.02 0.06 0.05 0.02 0.050 0.02 max Mn, max 1.50 1.50 1.50 1.50 1.50 1.50 1.00 1.00 1.50 1.00 1.00 1.00 1.00 1.5 1.00 1.0 max 1.00 Si, max 2.00 1.25 2.00 2.7-3.7 3.5-4.5 1.0-2.0 1.00 1.00 3.00 1.00 1.00 0.80 1.00 0.5 0.80 1.0 max 0.50 P, max 0.03 0.03 0.03 0.03 0.03 0.03 0.040 0.040 0.03 0.040 0.040 0.03 0.015 0.03 0.025 0.030 0.020 max S, max 0.03 0.03 0.03 0.03 0.03 0.03 0.030 0.030 0.03 0.030 0.030 0.03 0.015 0.03 0.025 0.030 0.020 max Cu 1.25 26.0- 26.0- 27.0- 27.0- 26.0- ... ... ... ... ... ... ... ... ... 1.50- ... max 33.0 33.0 33.0 33.0 33.0 3.50 Mo ... ... ... ... ... ... 26.0- 30.0- ... 16.0- 17.0- 15.0 8.0-10.0 2.0-3.5 12.5-14.5 2.5-3.5 15.0-16.5 30.0 33.0 18.0 20.0 -17.5 Fe 3.00 3.50 3.50 3.50 3.50 3.50 4.0-6.0 3.00 11.0 4.5-7.5 3.0 max 2.0 5.0 max 2.0 max 2.0-6.0 balance 1.50 max max max max max max max max max max Ni 95.00 balance balance balance balance balance balance balance balance balance balance balance balance balance balance 38.0- balance min 44.0 Cr ... ... ... ... ... ... 1.00 1.0 14.0- 15.5- 17.0- 15.0- 20.0-23.0 11.0-14.0 20.0-22.5 19.5- 22.0-24.0 17.0 17.5 20.0 17.5 23.5 A 494/A 494M – 03a Cb (Nb) ... 0.5 0.5 ... ... 1.0-3.0 ... ... ... ... ... ... 3.15-4.50 ... ... 0.60- ... max max 1.20 W ... ... ... ... ... ... ... ... ... 3.75- ... 1.0 ... ... 2.5-3.5 ... ... 5.25 max2 V ... ... ... ... ... ... 0.20- ... ... 0.20- ... ... ... ... 0.35 max ... ... 0.60 0.40 Bi ... ... ... ... ... ... ... ... ... ... ... ... ... 3.0-5.0 ... ... ... Sn ... ... ... ... ... ... ... ... ... ... ... ... ... 3.0-5.0 ... ... ... A Order M35-1 or M30C when weldability is required.
A 494/A 494M – 03a TABLE 2 Heat Treat Requirements Grade Heat Treatment CZ100, M35-1, M35-2, CY40 Class 1, M30H, M30C, As cast M25S Class 1, CY5SnBiM M25S, Class 2A Load into furnace at 600°F [315°C] maximum. Heat to 1600°F [870°C] and hold for 1 h plus an additional 30 min for each 1⁄2 in. [13 mm] of cross section over 1 in.B Cool to 1300°F [705°C]C and hold at temperature for 30 min then quench in oil to room temperature. M25S, Class 3 Load into furnace at 600°F [315°C] maximum. Heat slowly to 1100°F [605°C] and hold to develop maximum hardness. Furnace or air cool to room temperature. N12MV, N7M Heat to 2000°F [1095°C] minimum, hold for sufficient time to heat castings to temperature, quench in water or rapid cool by other means. CW12MW, CW6M, CW6MC, CW2M Heat to 2150°F [1175°C] minimum, hold for sufficient time to heat castings to temperature, quench in water or rapid cool by other means. CY40, Class 2 Heat to 1900°F [1040°C] minimum, hold for sufficient time to heat castings to temperature, quench in water or rapid cool by other means. CX2MW Heat to 2200°F [1205°C] minimum, hold for sufficient time to heat castings to temperature, quench in water or rapid air cool by other means. CU5MCuC Heat to 2100°F [1150°C] minimum, hold for sufficient time to heat castings to temperature, quench in water. Stabilize at 1725–1815°F [940–990°C], hold for sufficient time to heat castings to temperature, quench in water or rapid cool by other means. CX2M Heat to 2100°F [1150°C] minimum, hold for sufficient time to heat castings to temperature, quench in water or rapid air cool by other means. A M25S, while machinable in the “as cast” condition, is capable of being solution treated for improved machinability. It may be subsequently age hardened to the hardnessspeciﬁed in Table 3 and ﬁnished machined or ground. B For cross sections over 6 in. [125 mm] it may be necessary to increase the hold time if maximum softness is desired. C For maximum softness and the least variation in hardness levels, castings should be transferred from an oven at 1600°F [870°C] to a second oven at 1300°F [705°C]. 5.2.4 Marking-for-identiﬁcation requirements, if any (see 7.2 An analysis of each master heat shall be made by the13.1), and manufacturer to determine the percentages of the elements 5.2.5 Supplementary requirements desired, including the speciﬁed in Table 1. The analysis shall be made from astandards of acceptance. representative sample taken during the pouring of the master heat. Chemical composition shall be reported to the purchaser6. Heat Treatment or his representative. 6.1 Castings shall be heat treated in accordance with the 7.3 Test Methods E 76 or Test Methods E 354 shall be usedrequirements in Table 2. for referee purposes. Test Methods E 30 or Methods E 38 shall NOTE 1—Proper heat treatment of these alloys is usually necessary to be used if Test Methods E 76 or Test Methods E 354 do notenhance corrosion resistance and, in some cases, to meet mechanical include a method for some element present in the material.properties. Minimum heat treat temperatures are speciﬁed; however, it issometimes necessary to heat treat at higher temperatures, hold for some 8. Tensile Propertiesminimum time at temperature, and then rapidly cool the castings in order 8.1 One tension test shall be made from each master heatto enhance the corrosion resistance and meet mechanical properties. except for grades M25S and CY5SnBiM when the master heat 6.2 When Class 1 is speciﬁed, grades CY40 and M25S shall is used to pour the castings. One tension test shall be madebe supplied in the as-cast condition. When Class 2 is speciﬁed, from each melt except for grades M25S and CY5SnBiM. Testgrades CY40 and M25S shall be supplied in the solution- results shall conform to the tensile requirements speciﬁed intreated condition. When Class 3 is speciﬁed, grade M25S shall Table 3. Test bars shall be poured in special blocks from thebe supplied in the age-hardened condition. same heat as the castings represented. 8.2 The bar from which the test specimen is taken shall be7. Chemical Composition heat treated in production furnaces to the same procedure as the 7.1 These alloys shall conform to the chemical composition castings it represents. If the castings are not heat treated, therequirements prescribed in Table 1. bar used for the test specimen must not be heat treated. TABLE 3 Mechanical Properties CZ100 M35-1 M35-2 M30H M25S M30C N12MV N7M CY40 CW- CW6M CW2M CW6MC CY5S- CX2MW CU5- CX2M 12MW nBiM MCuCTensile strength, 50 000 65 000 65 000 100 00 ... 65 000 76 000 76 000 70 000 72 000 72 000 72 000 70 000 ... 80 000 75 000 72000 min, psi [MPa]               Yield strength, 18 000 25 000 30 000 60 000 ... 32 500 40 000 40 000 28 000 40 000 40 000 40 000 40 000 ... 45 000 35 000 39000 min, psi [MPa]               Elongation in 2 in. 10.0 25.0 25.0 10.0 ... 25.0 6.0 20.0 30.0 4.0 25.0 20.0 25.0 ... 30.0 20.0 40 [50 mm],A min, % BHardness HB ... ... ... ... ... ... ... ... ... ... ... ... ... ... ... ... A When ICI test bars are used in tensile testing as provided for in Speciﬁcation A 732/A 732M, the gage length to reduced section diameter ratio shall be 4 to 1. B 300 HB minimum for the age hardened condition. 3
A 494/A 494M – 03a 8.3 Test specimens may be cut from castings, at the produc- [65 cm2]. All other weld repairs shall be considered minor.er’s option, instead of from test bars. Major and minor weld repairs shall be subject to the same 8.4 When castings are produced by methods other than quality standards as are used to inspect the castings.investment process, tension test coupons shall be machined to 11.3 Castings of M30H, M25S, and CY5SnBiM may not bethe form and dimension shown in Fig. 8 of, and tested in weld repaired.accordance with, Test Methods E 8. 11.4 Grades N12MV, N7M, CW12MW, CW6M, CW2M, 8.4.1 When castings are produced by the investment pro- CX2MW, and CX2M may require post weld heat treatmentcess, test specimens in accordance with Speciﬁcation A 732/ after major weld repairs. If post weld heat treatment isA 732M shall be used for measurement of tensile properties. required, it must be speciﬁed along with the grade. If required, 8.5 If any specimen shows defective machining or develops it shall be performed in accordance with Section 6.ﬂaws, it may be discarded and another substituted from the 11.5 For grade CU5MCuC, the composition of the depos-same heats. ited weld metal shall be similar to that of AWS A5.14 ER 8.6 To determine conformance with the tension test require- NiCrMo3 or AWS A5.11 E NiCrMo3.ments, an observed value or calculated value shall be roundedin accordance with Practice E 29 to the nearest 500 psi [3.5 12. Rejection and RehearingMPa] for yield and tensile strength and to the nearest 1 % for 12.1 Samples that represent rejected material shall be pre-elongation and reduction of area. served for two weeks from the date of transmission of the rejection report. In case of dissatisfaction with the results of the9. Workmanship, Finish, and Appearance tests, the manufacturer may make claim for a rehearing within 9.1 Critical surfaces of all castings intended for corrosion- that time.resistant service shall be cleaned. Cleaning may be accom-plished by blasting with clean sand or metallic corrosion- 13. Product Markingresistant shot or by other approved methods. 13.1 Castings shall be marked for the material identiﬁcation with the ASTM speciﬁcation designation (A 494/A 494M) and10. Quality grade symbol, that is, CY40. The manufacturer’s name or 10.1 The castings shall not be peened, plugged or impreg- identiﬁcation mark and the pattern number shall be cast ornated to stop leaks. stamped on all castings except those of such small size as to 10.2 Internal chills and chaplets may be used in the manu- make such marking impractical. To minimize small defectsfacture of castings. However, the chills, chaplets and affected caused by dislodged particles of molding sand, the number ofcast material must be completely removed. cast identiﬁcation marks shall be minimized. The marking of heat numbers on individual castings shall be agreed upon by11. Repair by Welding the manufacturer and the purchaser. Markings shall be in such 11.1 Repairs shall be made by using a welding procedure position as not to injure the usefulness of the casting.and operators capable of producing sound welds. The compo- 13.1.1 When the castings are too small to mark individually,sition of deposited weld metal shall be similar to that of the a symbol traceable to the heat shall be placed on the castingscastings. and the required identiﬁcation then placed on a tag affixed to 11.2 Weld repairs shall be considered major in the case of a the container in which these castings are shipped.casting that has leaked on hydrostatic test or when the depth ofthe cavity after preparation for repair exceeds 20 % of the 14. Keywordsactual wall thickness, or 1 in. [25 mm], whichever is smaller, 14.1 corrosion resistant applications; nickel; nickel alloyor when the extent of the cavity exceeds approximately 10 in.2 castings; nickel alloys; nickel castings SUPPLEMENTARY REQUIREMENTS The following supplementary requirements shall not apply unless speciﬁed in the purchase order. A list of standard supplementary requirements for use at the option of the purchaser is included in Speciﬁcation A 781/A 781M. Those which are ordinarily considered for use with this speciﬁcation are given below; others enumerated in Speciﬁcation A 781/A 781M may be used with this speciﬁcation upon agreement between the manufacturer and the purchaser. 4
A 494/A 494M – 03aS2. Radiographic Examination The weld test to be used shall be agreed upon between the purchaser and manufacturer.S3. Liquid Penetrant Examination S22.1.1 Prepare and weld the test bar cast in accordanceS6. Certiﬁcation with Fig. 1 and in accordance with Fig. 3. S22.214.171.124 Machine the cast skin and unsound metal fromS10. Hardness Tests two adjacent faces of the as-cast specimen, exclude the riser S10.1 When composition M25S material is ordered with a face, and cut the specimen into approximately 6-in. [150-mm]hardness maximum or range in the as-cast or solution treated lengths.condition, hardness tests shall be made in accordance with Test S126.96.36.199 Clamp the two 6-in. [150 mm] lengths together toMethods and Deﬁnitions A 370. The test location, number of form a double V-joint and weld two passes at a time ontests, and hardness values shall be agreed upon between the alternate sides of the specimen using 1⁄8-in. [3-mm] diametermanufacturer and purchaser. electrodes that will deposit metal of similar composition of the S10.1.1 If castings are ordered in the as-cast condition, test pieces.hardness determinations shall be made on two different repre- S188.8.131.52 Allow the specimen to cool to room temperaturesentative areas of each casting or coupon selected for test. between passes, remove all ﬂux, and examine visually for S10.1.1.1 By agreement between purchaser and producer, cracks.those as-cast castings which fail to meet the required hardness S184.108.40.206 The clamps may be removed from the specimenmay be accepted in the solution annealed and hardened after the ﬁrst two weld passes have been completed.condition if the hardness thus developed meets the hardness S220.127.116.11 Deposit alternate series of passes until the doublerequirement of the speciﬁcation. V-groove has been completely ﬁlled. After the second series S10.1.2 If castings ordered are in the solution-treated con- (number 4 pass) a 5⁄32-in. [4-mm] diameter electrode may bedition, two sample castings or two coupons representing the lot used if desired.shall be heat treated for tests (see S10.1.1). Hardness determi-nations shall be made on two different representative areas of S18.104.22.168 During welding allow each pass to cool, clean,each casting or coupon. and examine visually for cracks. The presence of cracks shall S10.1.3 When hardness tests are made, the specimens shall be cause for rejection.be at least 1⁄4 in. [6 mm] in thickness and the area to be tested S22.214.171.124 Upon completion of the welding, cut one sectionshall be ground clean before the hardness tests are made. approximately 3⁄4 in. [19 mm] long transverse to the weld from each end and discard.S22. Weldability Test S126.96.36.199 Polish each end of the remaining center section on S22.1 If weldability tests are speciﬁed for M30C or M35-1, a 100/200-grit wheel and etch with concentrated HNO3 or withprepare a coupon obtained from a test bar shown in Fig. 1 or Lepito’s etchant. Prepare Lepito’s etchant as follows: (a) 15 gFig. 2 for each lot of composition M30C or M35-1 castings. of (NH4) 2SO4 dissolved in 75 cm3 of water; (b) 250 g of FeCl3(powdered) dissolved in 100 cm3 of HCl; (c) mix solutions (a) and (b) and add 30 cm3of HNO3. S188.8.131.52 Examine the etched section under low magniﬁca- tion (5 to 103). The lot represented by the test specimen shall be accepted if it complies with the following crack require- ments: (a) Three cracks maximum in linear inch of base metal and (b) The length of any crack in the base metal does not exceed 0.20 in. [5 mm]. S184.108.40.206 Cracks observed in the weld metal during the low-magniﬁcation examination shall not be cause for rejection. S220.127.116.11 Failure of welded test bars to comply with any of the requirements S22.1 through S18.104.22.168 shall result in rejection of the lot represented. S22.1.2 Prepare and weld the test bar cast in accordance with Fig. 2 as follows: S22.214.171.124 Fill the groove in the block completely with weld deposit using manual metallic arc process with 1⁄8-in. [3.2–mm] Metric Equivalents or 5⁄32-in. [4-mm] diameter electrodes that will deposit metal of similar composition of the test piece. in. 1 3 4 12 S126.96.36.199 Remove one 3⁄8-in. [10-mm] thick bend coupon [mm]     longitudinally from the welded block by machining, sawing, NOTE—Riser shall be machined off and 1 in. [25 mm] square by 12 in. abrasive cutting, or other suitable means. Make a transverse[305 mm] coupon shall be used for x-weld test. See Fig. 3. side bend test of the welded joint in accordance with Practice FIG. 1 Weld Test Bar (As Cast) A 488/A 488M. 5
A 494/A 494M – 03a Metric Equivalents in. ⁄ 14 38 ⁄ ⁄ 34 11⁄8 23⁄4 31⁄4 6[mm]        FIG. 2 Weld Test Bar (As Cast) S188.8.131.52 Remove a transverse weld macro-specimen from the welded plate and visually examine for cracks. This speci- men may be the same one to be used for the bend specimen. S22.1.3 Acceptance: S184.108.40.206 Cracks as tears in the casting in the fusion zone or heat-affected zone of the macro-specimen shall be cause for rejection. Cracks originating at the weld bead undercuts, at weld slag inclusions, or at casting defects shall not be cause for rejection. Metric Equivalents S220.127.116.11 Cracks or other open defects exceeding 1⁄8-in. [3.2 in. ⁄ 34 41⁄2 mm] measured in any direction on the convex surface of the [mm]   bent specimens shall be cause for rejection, except that cracks FIG. 3 X-Weld Test occurring on the corners while testing and cracks originating at weld bead undercuts shall not be considered. 6
A 494/A 494M – 03a SUMMARY OF CHANGES Committee A01 has identiﬁed the location of selected changes to this standard since the last issue (A 494/A 494M – 03) that may impact the use of this standard. (Approved Oct. 1, 2003)(1) Added new alloy CX2M. Committee A01 has identiﬁed the location of selected changes to this standard since the last issue (A 494/A 494M – 01ae1) that may impact the use of this standard. (Approved May 10, 2003)(1) Added UNS numbers to Table 1 and deleted them else- (2) Deleted the dashes in the alloy designations.where in the standard. ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or firstname.lastname@example.org (e-mail); or through the ASTM website (www.astm.org). 7